friction, wear, and adhesion characteristics of wear, and adhesion characteristics of...
Post on 16-Mar-2018
Embed Size (px)
-- NASA TECHNICAL NOTE TN D-3235 7- .-
FRICTION, WEAR, A N D
ADHESION CHARACTERISTICS OF
TITANIUM-ALUMINUM ALLOYS I N VACUUM
by Donald H. Buckley and Robert L. Johnson 1 Lewis Research Center
N A T I O N A L A E R O N A U T I C S A N D SPACE A D M I N I S T R A T I O N W A S H I N G T O N , D. 1 i 1[
TECH LIBRARY KAFB, NM
0079 8 09
FRICTION, WEAR, AND ADHESION CHARACTERISTICS O F
TITANIUM-ALUMINUM ALLOYS IN VACUUM
By Donald H. Buckley and Robert L. Johnson
Lewis Research Center Cleveland, Ohio
NATIONAL AERONAUTICS AND SPACE ADMINISTRATION
For sale by the Clearinghouse for Federal Scientific and Technical Information Springfield, Virginia 22151 - Price $1.00
FRICTION, WEAR, AND ADHESION CHARACTERISTICS OF
TITANIUM-ALUMINUM ALLOYS IN VACUUM
by Donald H. Buckley and Robert L. Johnson
Lewis Research Center
Friction, wear, and adhesion measurements were made in vacuum (lo- mm Hg) of titanium-aluminum alloys containing 11, 16, and 21 weight percent aluminum. Experi
3ments were conducted with a 16-inch-radius rider sliding on the flat surface of a 221-inchdiameter disk specimen at loads to 1500 grams. The disk was rotated to produce sliding velocities to 750 centimeters per second.
With increasing addition of aluminum to titanium, an increase in lattice ratio (c/a) for titanium occurred along with a decrease in friction, wear, and adhesion. The increase in (c/a) lattice ratio with the addition of aluminum to titanium occurred even though the unit cell s ize decreased; these results are unlike those with the addition of tin and oxygen to titanium. While titanium exhibited an adhesion coefficient of 5.3, the titanium-aluminum alloys exhibited adhesion characteristics which could be considered negligible.
These alloys exhibited superior friction and wear properties in vacuum compared with 52100 and 440-C stainless steels. Experiments were conducted with the alloys sliding on themselves and on 440-C stainless steel. Friction was less for the alloys sliding on 440-C stainless than when sliding on themselves.
Marked differences in adhesion, friction, wear, and welding tendencies are found for metals with different crystal structures (refs. 1 to 5). Those metals possessing hexagonal crystal structures or polymorphic metals in the hexagonal form exhibit lower friction, wear, and adhesion characteristics than cubic metals or polymorphic metals in the cubic form. Further, with the hexagonal metals which exhibit the lower friction and wear characterist ics, a dependence upon lattice parameters is found (ref. 5). Those hexagonal
metals possessing near ideal sl ip behavior (basal slip) have lower friction characteristics than those exhibiting prismatic and pyramidal sl ip (Ti, Zr, and Hf) (ref. 5).
With metals such as titanium, the addition of alloying elements which expand the crystal lattice in the C-axis direction (increased c/a ratio) results in a decrease in friction coefficient. Elements such as tin and oxygen have this effect upon titanium; they increase the c/a lattice ratio by increasing the C-axis (ref. 6).
There are, however, elements which increase the c/a lattice ratio even though the individual lattice parameters (c and a) decrease with increasing amount of alloying element. That is, the unit hexagonal cell is decreasing in s ize but the rates of decrease of c and a with addition of alloying element a r e such that the ratio c/a increases. An example of such an alloy system is aluminum in titanium.
If the significant parameter is lattice ratio c/a, the addition of aluminum to titanium should do more to reduce friction, wear, and welding tendencies of titanium than tin and oxygen. With decreasing unit cell size, an increase in atomic packing density will occur. The influence of atomic density on friction at this time is not known. An attractive feature of aluminum as an alloying element with titanium is that the alloy itself would have low density. (Light weight is an important consideration in aerospace devices. )
This investigation was conducted to determine in a vacuum environment whether the lattice ratio c/a o r the interatomic distance along the C-axis in the hexagonal metal titanium is of primary importance in determining the friction characteristics of titanium. Crystallographic considerations would indicate that the ratio c/a is the important parameter since sl ip mechanisms in hexagonal crystals depend upon it. The experiments of this study were conducted with aluminum alloyed in titanium. Since aluminum increases the c/a ratio of titanium with a decrease in unit cell size and data exist for systems which expand the C-axis (titanium- oxygen and titanium-tin), the factor responsible for a decrease in friction characteristics with such alloy additions can be resolved.
The experiments of this investigation were conducted with a hemispherical r ider specimen sliding on a flat disk surface. All experiments were made at a pressure of lo- millimeter of mercury o r lower to reduce the presence of surface contaminents. Friction, wear, and adhesion measurements were made with titanium as well as with titanium-aluminum alloys. Adhesion measurements were made with copper for reference purposes.
The titanium-aluminum alloys used in this investigation were all arc-cast under argon at reduced pressure. Small pieces of the metals to be cast were placed in a water-cooled copper mold and arc-melted with a tungsten electrode. The casting was then turned over in the mold and remelted. This process was repeated a number of t imes to ensure homo
geneity in the casting. After the alloys cooled, they were removed and metallographic and chemical analyses were made. Friction and wear specimens were then prepared. In or der to ensure that the structure was primarily hexagonal rather than cubic (alpha rather than beta), all samples were sealed in evacuated tubes and heat-treated at 1400' F (760' C) for 72 hours.
I APPARATUS AND EXPERIMENTAL PROCEDURE
The apparatus used in this investigation is shown in figure 1. The basic elements of 3the apparatus were the test specimens (a 221-in. -diam. flat disk and a 16-in. -rad. rider)
mounted in a vacuum chamber. The disk specimen was driven through a magnetic drive coupling. The coupling consisted of two 20-pole magnets spaced axially 0.150 inch apart with a 0.030-inch diaphragm between magnet faces. The drive magnet outside the vacuum system was coupled to a hydraulic motor. The driver magnet was completely enclosed with a nickel-alloy housing (cutaway in fig. 1) and was mounted at the upper end of the shaft within the chamber. The disk specimen was at the lower end of the shaft.
The rider specimen was supported in the specimen chamber by an a r m mounted by gimbals and sealed by a bellows to the chamber. A linkage at the end of the retaining a r m away from the r ider specimen was connected to a strain-gage assembly. The assembly was used to measure frictional force. Load was applied through a dead-weight loading system. Directly opposite the load (at 180') was a strain-gage assembly for measuring adhesion forces.
Attached to the lower end of the specimen chamber was a 400-liter-per-second ionization pump and a vac-sorption forepump. The pressure in the chamber adjacent to the specimen was measured with a cold-cathode ionization gage. Also present in the apparatus was a diatron-type mass spectrometer (not shown in fig. 1)for determination of gases present in the vacuum system. A 20-foot, 5/16-inch-diameter stainless-steel coil was used for liquid-nitrogen and liquid-helium cryopumping of the vacuum system.
The vacuum chamber and specimens were baked out at 200' C for 16 hours prior to , each experiment. In the adhesion experiments with copper, the specimen was heated to
400' C with an electron gun to drive off and dissociate surface adsorbates and oxides. The adhesion coefficient (ratio of breakaway load to applied load) was determined
after the friction studies were completed. The rotating drive was stopped and the specimens were left in contact under load for 90 minutes. Then a small drive motor with a strain-gage assembly (fig. 1)was used to separate the specimens, and the force required was recorded on a s t r ip chart.
SPECIMEN FINISHING AND CLEANING PROCEDURE
The disk and rider specimens used in the friction and wear experiments were finished to a roughness of 4 to 8 microinches. Before each experiment, the disk and rider were given the same preparatory treatment: (1)a thorough rinsing with acetone to remove oil and grease, (2) a polishing with moist levigated alumina on a soft polishing cloth, and (3) a thorough rinsing with tap water followed by distilled water. For each experiment, a
I new set of specimens was used.
RESULTS AND DISCUSSION
Crystal Forms of Ti tanium
Titanium alloys exist in a number of forms. These a r e alpha-stabilized (hexagonal crystalline form), beta-stabilized (cubic crystalline form), and alpha-beta alloys in which a mixture of the two crystalline forms exist. The cubic form (beta titanium) is often selected for structural uses because of improved strength characteristics. For slider materials use, the chief criterion has been hardness.
In reference 4 the addition of tin and oxygen (alpha stabilizers) to titanium was found to reduce friction markedly. Both alloying elements expanded the lat